Swelling effects in cross-linked polymers by
Andrzej Sienkiewicz1 Patrycja Krasucka1 Barbara Charmas2
Received: 17 November 2016 / Accepted: 25 January 2017 /
Published online: 22 February 2017
The Author(s) 2017. This article is published with open access
Abstract The present study focuses on the mechanism of
swelling and evaluates interactions between solvents of
different chemical characters (polarethanol, nonpolar
n-heptane) and commercially available porous Amberlite
polymers (XAD4, XAD16, XAD7HP) by temperature-
programmed desorption (TPD). The first two polymers are
the product of copolymerization of styrene and divinyl-
benzene. Despite having the same chemical composition,
they differ in pore size and volume. The Amberlite
XAD7HP is composed of an acrylic matrix and has lower
pore volume and specific surface area than XAD16 and
XAD4. All three resins have the ability to swell, though the
per cent of polymeric network expansion during this pro-
cess varies depending on the solvent used (e.g. in
orthosilicate, XAD4 and XAD16 spherical particles
increase in volume by 2030%, while XAD7HP particles
can expand by more than 120%). The TPD experiment was
performed in dynamic linear and quasistatic heating mode.
Based on thermogravimetric data, the desorption energy of
selected liquids and pore size distribution in the swollen
state were estimated. The obtained results are discussed in
terms of both mathematical modelling and low-temperature
nitrogen adsorptiondesorption experiment.
Keywords Amberlite resins Swelling Ethanol n-Heptane Porous
polymer Desorption energy
The swelling process is, by definition, an increase in the
volume of a gel or solid connected with the uptake of a
liquid or gas . The absorption of liquids leads to
in the mechanical properties of the swollen material and
may create extra pressure when it occurs in confined
spaces, which results in various deformations of the
swollen material (i.e. surface creases and wrinkles) .
The discussed process may also significantly alter adsorp-
tiondesorption properties of adsorbates [5, 6]. In polymer
dissolution, swelling is the first step in the interaction
between liquid molecules and polymeric network, which is
usually followed by solvatation of polymer chains. The
immersion of cross-linked polymers in solvents does not
lead to their dissolution because of their chemically bonded
hydrocarbon chains; nonetheless, these links do not prevent
cross-linked polymers from swelling.
The first comprehensive approach to quantitatively
describing the process of swelling of nonporous materials
was presented in the FloryRehner theory . In this the-
ory, the rate of maximum swelling is the result of the
equilibrium between two major adverse effects: the entropy
of mixing and the entropy of polymer chain configuration.
For quantitative determination of interactions between
liquid molecules and polymeric chains, the FloryHuggins
parameter was proposed; unfortunately, it cannot be
applied in every case .
Historically, swelling was estimated by a weight method
or by linear method with the use of the cathetometer. Both
these methods require swollen particles to be in
& Andrzej [email protected]
1 Department of Adsorption, Faculty of Chemistry, Maria
Curie Skodowska University, Maria Curie-Skodowska sq. 3,
20-033 Lublin, Poland
2 Department of Chromatographic Methods, Faculty of
Chemistry, Maria Curie Skodowska University, Maria
Curie-Skodowska sq. 3, 20-033 Lublin, Poland
J Therm Anal Calorim (2017) 130:8593
equilibrium with the solvent; neither of them is suitable
measuring the swelling of polymer particles in volatile
liquids (e.g. ethanol, heptane). In the present study, for
convenience and reproducibility of the presented results,
instead of either of the above-mentioned methods, tem-
perature-programmed desorption and microscopic mea-
surements were used.
In the current research, three commercially available
cross-linked porous Amberlite resins: XAD4, XAD16 and
XAD7HP, immersed in ethanol and in heptane, were
investigated. These materials are widely used as sorbents
, ionites  and organic frameworks for composite
synthesis . Their insolubility and resistance to both
acids and bases, along with their high sorption capacity,
makes them very versatile materials. The degree of poly-
meric network expansion depends on the pore structure of
Amberlite and on the chemical character of solvent mole-
cules. Swelling affects their mechanical properties at the
same time altering their ability to recover adsorbed sub-
stances . These problems are particularly important in
the case of porous polymers. Porosity is, next to the
chemical character, the main feature of widely used poly-
mer materials employed in separation sciences and
adsorption. However, swelling of porous polymers is rarely
investigated because of the complexity of the process. The
uptake of solvent is in this case a combination of capillary
action and the swelling of polymer matrix. A thermo-
gravimetric experiment allows the evaluation of both these
effects separately and provides sufficient information for
better understanding of the adsorption and swelling of
All three Amberlite resins: XAD4, XAD16 and XAD7HP
referred further as XAD7, purchased from SigmaAldrich,
were thoroughly washed with redistilled water up to the
point where no chloride ions were detected in the eluent
the manufacturer provides spheres immersed in sodium
chloride solution. Subsequently, polymeric material was
dried in a regular dryer at 353 K for minimum 12 h and in
a vacuum dryer for another 4 h at the same temperature.
Anhydrous ethanol (99.8%) and n-heptane both pure p. a.
were purchased from POCH, Poland, and used without any
The low-temperature nitrogen adsorptiondesorption
experiment carried out with a volumetric adsorption
analyser, ASAP 2405 (Micromeritics), provided data for
calculation of the specific surface area (SBET, from BET
method, p/p0 from 0.05 to 0.25) , the total pore volume
(Vp, at p/p0 = 0.995) and the pore size distribution (PSD,
from BJH procedure) .
Temperature-programmed desorption was performed
using Derivatograph-C (MOM, Hungary), Paulik & Paulik
system. The linear mode at three heating rates (1, 5 and
10 K min-1) was employed to desorb ethanol and n-hep-
tane from selected Amberlite resins (mass of swollen
polymer was approximately 100 mg). Additionally, solvent
desorption was conducted in quasistatic mode (level
0.3 mg; Qp0.5 K min-1).
The dimensions of the swollen particles were measured
with Nikon SMZ1500 optical microscope.
Results and discussion
All the three Amberlite polymers selected for the study are
in the form of white opaque spheres. The diameter of these
particles ranges from 200 to 600 lm. Parameters charac-terizing
the porosity of polymers were obtained with the
use of low-temperature nitrogen adsorptiondesorption
experiment (Fig. 1; Table 1).
Low-temperature adsorptiondesorption of the selected
Amberlite polymers reveals that N2 adsorbs reversibly on
dried cross-linked polymers. Adsorption isotherms for each
of them consist of a hysteresis loop whose shape for XAD4
and XAD7 may indicate that the formed pores have the ink
bottle shape (plateau followed by sudden decrease on
1 , S
Fig. 1 Low-temperature adsorption (filled figures)desorption
(openfigures) of nitrogen for XAD4 (triangles), XAD16 (squares)
86 A. Sienkiewicz et al.
desorption curve) , whereas adsorption branch shows
monotonous increase in the whole pressure range.
SBET, Vp and DPSD in brackets are the values obtained
from our previous N2 adsorptiondesorption measurements
. The differences in values of porosity parameters may
result from different batches of material and different
instruments used in the studies
To examine the degree of swelling of all characterized
materials in two different solvents polar (ethanol) and
nonpolar (n-heptane), optical microscope measurements
The dimensions of the dry and swollen polymeric spheres
were measured from images obtained from an optical
microscope (Fig. 2). As it may be seen, the change in the
appearance of the spheres after the transition from the dry
and the swollen state is noticeable. Dry particles have
opaque white colour, while spheres immersed in liquid are
translucent. This qualitative change is shared by all three
materials, but the increase in volume in the case of XAD7
is the most noticeable of them all.
On the basis of microscope imaging, it may be seen that
Amberlite polymer particles swell isotropically (wetted
particles maintain the spherical shape of dry beads). From
the measured diameter, radius (r) was obtained and used to
calculate the volume of the bead (Vb. = 4/3pr3). Sincethere is
slight difference between swelling of relatively
large and small particles, the sum of volumes of at least 25
spheres was taken into account and compared. From this
comparison, the increase in volume, expressed as the
swelling ratio (S = 100% 9 (Vsp - Vd)/Vd, where Vsp
the volume of swollen particles and Vdvolume of dry
particles), was calculated and is presented in Table 2.
On the basis of the data collected in the table, as well as
previous studies , it may be concluded that the mod-
erately polar XAD7 matrix exhibits a much higher swelling
capacity (the swelling ratio higher than 100%) in both polar
and nonpolar solvents than hydrophobic polymers. What is
more, polar XAD7 in n-heptane swells noticeably more
than it does in ethanol. This phenomenon can be explained
by the fact that the uptaken n-heptane molecules are
located in the vicinity of polymeric hydrocarbon chains.
Thus, n-heptane molecules, tightly packed around poly-
meric chains, force them to extend more. Astonishingly,
the difference in swelling between XAD4 and XAD16 was
observed. Despite the same chemical composition, the
more porous XAD16 (with larger specific surface area and
extremely large pore volume) has a greater ability to
expand than the less porous XAD4.
Temperature-programmed desorption of heptane and
ethanol provided TG and DTG curves (Fig. 3).
Thermogravimetric curves show that the imbibed liquid
constitutes from 50 up to 70% of the swollen polymer
mass. What is surprising, the material that swells the most
(XAD7) has only 50% w/w of the solvent, whereas
XAD16, for which the increase in volume is moderate but
which has the highest specific surface area, has liquid
uptake at level of 70% w/w. It is obvious that the total
desorbed amount of the solvent is the sum of the solvent
entrapped between the polymer chains and the solvent
present inside the pores. This conclusion can be supported
by weakly resolved peak on the slope of DTG curve only
for XAD16. Thus, the liquid desorbed from the pores,
especially wider ones, may be assumed as the part of bulk
liquid which is easily desorbed.
From the peak of the desorption on DTG curves, the
maximum temperature of desorption (Tp) was noted. With
the heat rate (b) and Tp known, it is possible to
estimatedesorption energy of heptane and ethanol from the
polymer using Amenomiya and Cvetanovic  equation:
2303RTp log EdA0
where Edenergy of desorption (kJ mol-1), A0quantity
adsorbed, Cconstant (related to desorption rate) and R
gas constant. Plotting linear function logT2pb
Table 1 Porosity parameters (SBETspecific surface area, Vppore
volume, DPSDthe diameter at the peak of PSD, D =
4Vp/SBETaveragepore diameter), dipole momentum (q)  and density
(d) of Amberlite resins
Amberlite SBET/m2 g-1 Vp/cm
3 g-1 DPSD/nm D/nm q/D d/g cm-3
6.0 0.3 1.08
8.1 0.3 1.08
4.9 1.7 1.24
Swelling effects in cross-linked polymers by thermogravimetry
can calculate the desorption energy from the coefficient of
the variable by a simple mathematic transformation. In all
the measured cases, the coefficient of determination of the
above-mentioned function is higher than 0.9. Obtained
values are presented in Table 3.
The obtained values of desorption energy (Ed) in both
cases are substantially higher than those for vaporization
pure liquid (42.3 kJ mol-1 for ethanol , 36.3 kJ mol-1
for heptane ). Pore dimensions and intermolecular
interactions play a crucial role in the estimation of des-
orption energy. These two factors may sum up or overlap
and compensate themselves. The narrowing of pore
diameter and establishing solventpolymer interactions
during the swelling will result in the increase in the total
energy needed for solute desorption. In the case of n-hep-
tane, which is unable to establish polar interactions with
Amberlite resins, the presence of liquid meniscus curvature
in the pores will be the key feature affecting the Ed value.
As shown in Table 3, the energy required for n-heptane
desorption increases along with specific surface area and
pore volume of the chosen Amberlites (XAD16[XAD4[XAD7).
According to the Kelvin equation, thelarger the liquid meniscus
radius is, the less energy is
needed to the occurrence of liquidgas transition. Thus, the
obtained Ed values may indicate that, although pore
dimensions in swollen material under study are changed,
the shape of the pores is preserved. In the case of ethanol,
the estimated desorption energy sequence is different than
that for heptane (XAD16[XAD7[XAD4). XAD7,which has smaller
specific surface area and pore volume
than the less polar XAD4, has a noticeably higher Ed value.
This is probably due to the dipoledipole interaction
between ethanol and XAD7 chains. Moreover, a great
ability of XAD7 matrix to swell in both ethanol and n-
heptane is a crucial factor, which probably contributes to
the rise of the desorption energy. Namely, during swelling,
solvent molecules are located inside and between poly-
mer chains (occupying every sterically available inner
polymer spaces), which hinders their desorption. Interest-
ingly, XAD16, less polar than XAD7, has the highest
desorption energy value. This could be caused by the
extreme uptake of ethanol (70% w/w) by the highly porous
XAD16 matrix. The diameter of XAD16 pores is twice as
large as it is for XAD4 and three times larger than it is
XAD7. Thus, the molecules of ethanol, smaller than n-
heptane, penetrates XAD16 matrix more easily, completely
filling pores and establishing dipoldipol interactions
between ethanol molecules within the pores.
The thermal desorption experiment for the same systems
was repeated in quasi-isothermal conditions using the
heating programme incorporated into Derivatograph.
Experimental curves, which may be assumed as isobars of
desorption measured in this specific heating mode, are
shown in Fig. 4.
TG curves presented above have a characteristic shape.
At the beginning of desorption, the temperature of the
material is too low to observe mass loss (approximately
horizontal line). After reaching the boiling temperature of
the solvent at quasistatic desorption programme, a vertical
line is registered. The mass loss on TG curve above the
boiling temperature represents the liquid that evaporates
from the sample, i.e. the amount of the solvent absorbed
Fig. 2 Image of dry (a, c) and swollen in ethanol (b) and in
heptane(d) spheres of XAD7. Red circle marks dry bead dimension.
Scale barfor (b) is the same as for (a) and (d) as for (c). (Color
Table 2 The swelling ratio (S) of the swollen Amberlites in
ethanol and in n-heptane presented with the standard deviation and
the confidenceinterval at 95% confidence level (CI)
Amberlite Ethanol n-Heptane
S/% CI S/% CI
XAD4 17.0 5.4 (14.8, 19.1) 28.5 4.1 (26.9, 30.1)
XAD16 40.7 2.7 (39.7, 41.7) 36.0 2.5 (35.0, 37.0)
XAD7 137.0 4.3 (135.3, 138.6) 149.0 5.6 (146.8, 151.2)
88 A. Sienkiewicz et al.
between polymer chains and inside pores. In other words,
the desorbed liquid represents the total amount of the
present in the sample. However, for a relatively small
swelling ratio (much lower than 50%) it may be assumed
that the released solvent in TG experiment represents the
solvent filling the pores (Fig. 5).
Knowing the amount of liquid evacuated above its
boiling point, pore size distributions for XAD4, XAD16
(Fig. 5) and XAD7 in swollen state were estimated using
the Kelvin equation and converting mass loss versus tem-
perature to volume loss versus pore radius  and
after differentiation of these curves. Taking into account
the amount of the liquid adsorbate desorbed above its
normal boiling point, the total pore volume of the polymers
Because of an extremely high swelling ratio for XAD7
and a great share of solvent taking part in the swelling, it
impossible to obtain reasonable PSD values. This phe-
nomenon can be explained by two causes. Firstly, the
expanding polymeric matrix results in diminishing free
inner spaces of the pore. The second cause might be related
to the fact that during the TG desorption, a very small
amount of the liquid is still adsorbed on pore walls and
forms a surface film of some thickness. The desorption of
the solvent represents the deswelling process and takes
place, in this case, in the range of 1.5 C. Any calculationsin
such a narrow temperature range are vitiated by errors.
The sharp decrease in the solvent mass on TG curves is, in
this case, registered without the characteristic inflection
points, which indicates that the solvent is evacuated
simultaneously from whole system. The shape of TG
curves for XAD4 and XAD16 Amberlites is much more
Temperature/K400 440 320 360
121 K min1
5 K min110 K min1
1 K min1
5 K min1
10 K min1
(a) (b)Fig. 3 TG (black lines) andDTG (red lines) curves for
XAD4, XAD16, XAD7
recorded at three different
heating rates 1 K min-1 (solid
line), 5 K min-1 (dashed line)
and 10 K min-1 (dotted line)
for desorption of ethanol (a) andn-heptane (b). (Colorfigure
Table 3 Estimated desorption energies (Ed) for ethanol and
Amberlite Ed/kJ mol-1
XAD4 58.5 51.9
XAD16 77.9 59.4
XAD7 66.6 48.9
Swelling effects in cross-linked polymers by thermogravimetry
useful for pore estimation. The desorption curve is less
steep and extended along the temperature axis, which
facilitates the calculations of PSD. The pore size distribu-
tion estimated from n-heptane and ethanol desorption
experiments is much narrower than it is for N2 adsorption,
and the values of peak maximum for both used liquids are
shifted towards smaller pore radius.
As it may be seen, PSD peaks maxima for n-heptane
desorption for both polymers are in a reasonable correla-
tion with the peak maximum obtained from the liquid
nitrogen desorption experiment. However, for ethanol
desorption, this difference is larger. This can be explained
by the fact that plot of the radius (calculated from the
Kelvin equation) versus temperature for alcohols (i.e.
ethanol) is much steeper than it is for hydrocarbons (graph
not shown). Thus, an error in estimating PSD using this
method is more pronounced for ethanol than it is for n-
The macroscopic increase in the volume of polymer during
liquid uptake is a result of both pore geometry change and
the elongation of polymeric matrix. Each polymer has a
certain ratio of free spaces (pores) to polymer skeleton. In
other words, cross-linked polymer may be considered as a
structure that consists of multiple pores with certain pore
wall thickness. For porous polymers during isotropic
increase in volume, the swelling ratio will affect pore wall
thickness and its length. Along with the expanding, the
polymer skeleton volume of free spaces between pore walls
will diminish proportionally to the degree of the polymer
expansion, which in turn is proportional to the amount of
the polymer specimen forming the pore walls. It is very
difficult to determine the thickness of pore walls in a dry
50 100 150 200
Fig. 4 TG curves gathered in isobaric mode for desorption of
ethanol(a) and n-heptane (b)
0 2 4 6
0 4 8 12 16 20
Fig. 5 Comparison of pore size distribution for XAD4 (a)
andXAD16 (b) obtained by low-temperature liquid nitrogen
adsorptiondesorption experiment (black dotted line) and derived
(blue solid line) and heptane (purple dashed line)
desorption data. (Color figure online)
90 A. Sienkiewicz et al.
and in a swollen state. For illustrative purposes and model
calculations, the volume ratio of pore volume in a dry
state to the pore volume in a swollen state was taken into
account (VS=VN2 ). VN2 value is known from N2 adsorption
experiment and VS is determined as the pore core volume
after the thickening of pore wall. Model calculations for
cylindrically shaped pores at different swelling ratios are
presented in Fig. 6 for ethanol (Fig. 6a) and n-heptane
In calculations, the thickness of walls was assumed to
fall within a wide range from 0.2 to 50 nm. The shape of
these curves is independent of the pore length. For strictly
geometrical reasons, these simulation calculations are valid
for materials whose swelling ratio does not exceed 200%.
In this model, it means that pores are completely closed
and the expansion of pore walls exceeds the pore space.
In real systems, knowing the swelling ratios, one can
estimate the characteristic point corresponding to the
specific degree of pore filling. For the studied polymers,
location of this point is different. In the case of XAD7
swollen in ethanol, the volume ratio (VS/VN2 ) is close to
It means that in its swollen state, this polymer has no free
volumes representing pores. For n-heptane VS/VN2 equal to
0.3 suggests that some volumes (outside the polymer skele-
ton) are present even with the total saturation of XAD7 with
the swelling agent. In the case of two hydrophobic polymers,
XAD4 and XAD16, relatively large values of VS/VN2 indi-
cate that there are free volumes in the samples, which do
take part in swelling and which may be ascribed to the pores
in the swollen state. It is worth mentioning that the
pore volumes are in wet samples filled with solvent. The
results presented in Fig. 6 are numerically expressed in
Table 4. Solvent volumes in column II of Table 4 are an
integral part of the total particle volume being the sum of
solvent, polymer and pore volumes.
The swelling ratio for XAD7 and the difference in the
volume of the solvent taking part in swelling, the latter of
which was obtained from TG experiment (the height of the
TG curve segment above the boiling point) and from a
simple calculation which took into account the solvent
uptake from mass of the polymer, are practically equal, and
consequently, VS/VN2 is close to zero. It means that the
volume accessible for ethanol outside the polymer matrix is
in this case occupied by the swollen polymer matrix. For
remaining polymers, this difference is more pronounced, as
it is depicted in Table 4 (column II and V) and points in
Fig. 6. VS/VN2 values are relatively high and reach maxi-
mum for XAD4 sample.
The presented calculations are the result of TG data
fitting to the model pore system characterized by low-
temperature nitrogen adsorption experiment and micro-
scopic observation of swelling expressed in swelling ratio
value. The results clearly indicate that a high swelling
results in the elimination of pores accessible for solvent
molecules. The whole internal pore system existing in a dry
sample is filled with the swollen polymer skeleton. At
lower swelling ratios, there remain pores which may be
assumed as a free space filled with solvent. This conclusion
is supported by the comparative study of pore volumes
estimated from nitrogen adsorption data with those calcu-
lated from TG experiment.
If it is assumed that the total desorbed amount of solvent
above the boiling point originates from pores, its volume
should be equal to the pore volume derived from adsorption
isotherm. Pore volumes calculated in that manner described
above are listed in Table 5. Extremely high difference in
pore volumes VSE and VN2 occurs in the case of XAD7
Amberlite. Pore volumes estimated by two different methods
are similar for XAD4 and XAD16 sample. This undoubtedly
indicates that small swelling degree favours the existence
free space in porous polymer which may accommodate quite
a large amount of the solvent.
Fig. 6 The relation of Vs/VN2 against the ratio of pore radius
to porewall thickness RN2 /WT for different swelling ratios (S); a
ethanol, b n-heptane. Curves 1, 2 and 3 correspond to Amberlite
and XAD16. Shaded area illustrates the relation of Vs/VN2 versus
WT in the range of S from 5 to 250%
Swelling effects in cross-linked polymers by thermogravimetry
Numerous studies of materials that have the ability to swell
in polar and nonpolar liquids were conducted with the TG
analysis (e.g. organic copolymers  and various
hydrogels ), but to our knowledge it is the first
reported approach to pore size distribution estimation in
swollen cross-linked polymers with the employment of
thermogravimetric analysis combined with microscopic
measurements. A standard procedure based on quasi-
isothermal programme of heating applied for desorption of
liquid from porous solid and the Kelvin equation, along
with a simple mathematic calculation, provides informa-
tion concerning free spaces in the swollen material. Ther-
mogravimetry results coupled with nitrogen adsorption
data provide valuable information on the solvent uptake
and make it possible to evaluate the share of polymer
swelling and pore system filling in total solvent
Attention has to be paid to initial porosity of the polymer
and intermolecular interactions between the polymer and
the solvent. Studies using TG technique facilitate investi-
gation of polymer pores in the swollen state. Amberlite
XAD7HP swells more than Amberlite XAD4 and XAD16
in both ethanol and n-heptane. Preliminary results of PSD
calculations on the basis of TG data show similar pore size
distributions in swollen particles as those calculated from
nitrogen adsorption data but with pore radius shifted to
lower values. In other words, the dimensions of pores in
swollen materials are smaller than in the dry state. An
increase in liquid uptake by Amberlite resins and swelling
rate depends not only on the chemical composition of the
polymer but also, to a great extent, on its porosity. The
calculations presented here contain several simplifications;
however, the correlation between macroscopic effects,
thermogravimetric measurements and those predicted by
model calculations is surprisingly satisfactory.
Open Access This article is distributed under the terms of the
CreativeCommons Attribution 4.0 International License
commons.org/licenses/by/4.0/), which permits unrestricted use,
bution, and reproduction in any medium, provided you give
credit to the original author(s) and the source, provide a link
Creative Commons license, and indicate if changes were made.
1. IUPAC. Goldbook. http://goldbook.iupac.org/S06202.html.
2. Hong W, Zhao XH, Suo ZG. Formation of creases on the
of elastomers and gels. Appl Phys Lett. 2009. doi:10.1063/1.
3. Chan EP, Smith EJ, Hayward RC, Crosby AJ. Surface
for smart adhesion. Adv Mater. 2008;20(4):711. doi:10.1002/
4. Guvendiren M, Burdick JA, Yang S. Kinetic study of
induced surface pattern formation and ordering in hydrogel
with depth-wise crosslinking gradient. Soft Matter.
5. Udoetok IA, Dimmick RM, Wilson LD, Headley JV. Adsorption
properties of cross-linked cellulose-epichlorohydrin polymers
aqueous solution. Carbohyd Polym. 2016;136:32940. doi:10.
6. Tran NB, Kim JY, Kim YC, Kim YJ, Kim JH. CO2-responsive
swelling behavior and metal-ion adsorption properties in
histamine-conjugated polyaspartamide hydrogel. J Appl Polym
Sci. 2016;. doi:10.1002/app.43305.
7. Flory PJ, Rehner J Jr. Statistical mechanics of
polymer networks II: swelling. J Chem Phys. 1943;.
8. Rogers CE, Stannett V, Szwarc M. The sorption of organic
vapors by polyethylene. J Phys Chem-Us. 1959;63(9):140613.
9. Blackadder DA, Keniry JS. Morphological consequences of
annealing high-density polyethylene in solvents. J Appl
Sci. 1972;16(5):1261. doi:10.1002/app.1972.070160517.
10. Brockmeier NF, Mccoy RW, Meyer JA. Gas-chromatographic
determination of thermodynamic properties of
2. Semicrystalline polymer systems. Macromolecules.
Table 4 Parameters characterizing polymers under study in
swollen state; VSE = Vpolymer 9 S%, where Vpolymer =
mpolymer/dpolymer; VS =VTG - VSE, where VTG is a solvent volume
desorbed above boiling point; RS = RN2 9 VS/VN2
Adsorbate Ethanol n-Heptane
VSE/cm3 g-1 VS/VN2 Rs/nm VSE/cm
3 g-1 VS/VN2 Rs/nm
XAD4 0.165 0.7579 4.6 0.276 0.6754 4.2
XAD7 1.113 0.0662 0.6 1.209 0.2698 1.5
XAD16 0.394 0.6805 8.3 0.349 0.6457 8.3
Table 5 Pore volumes for dry and swollen material (VTG). VSE
forTG data was calculated from the mass of solvent desorbed
Amberlite Pore volume/cm3 g-1
N2 adsorption TG experiment
XAD4 1.22 1.09 1.10
XAD16 1.85 1.66 1.55
XAD7 0.56 1.15 1.36
92 A. Sienkiewicz et al.
11. Lee SC, Yeo SM. Role of dilute polymer solution in
extraction by emulsion liquid membranes. J Ind Eng Chem.
12. Edebali S, Pehlivan E. Evaluation of Cr(III) by
resins from aqueous solution: equilibrium, thermodynamics
kinetics. Desalin Water Treat. 2014;52(3739):714353. doi:10.
13. Kierys A, Dziadosz M, Goworek J. Polymer/silica composite
core-shell type by polymer swelling in TEOS. J Colloid
Sci. 2010;349(1):3615. doi:10.1016/j.jcis.2010.05.049.
14. Yuan W, Wiehn M, Wang YC, Kim HW, Rittmann BE, Nielsen
DR. Solid-phase extraction of long-chain fatty acids from
ous solution. Sep Purif Technol. 2013;106:17. doi:10.1016/j.
15. Brunauer S, Emmett PH, Teller E. Adsorption of gases in
timolecular layers. J Am Chem Soc. 1938;60(2):30913. doi:10.
16. Barrett EP, Joyner LG, Halenda PP. The determination of
volume and area distributions in porous substances. 1.
tations from nitrogen isotherms. J Am Chem Soc. 1951;73(1):
17. Sigma-Aldrich. Product information. Amberlite XAD
18. Krasucka P, Stefaniak W, Kierys A, Goworek J.
composites and silicas produced by high-temperature
of organic component. Thermochim Acta. 2015;615:4350.
19. Amenomiya Y, Cvetanovic RJ. Application of
method to catalyst studies. 1: ethylene-alumina system. J
Chem. 1963;67(1):144. doi:10.1021/j100795a035.
20. NIST. WebBook. Ethanol.
21. NIST. WebBook. Heptane.
22. Paulik J, Paulik F, Arnold M. The derivatograph-Ca
puter-controlled simultaneous TG, DTG, DTA, TD and EGA appa-
ratus. I. J Therm Anal. 1987;32(1):3019.
23. Paulik F. Special trends in thermal analysis. New York:
24. Goworek J, Stefaniak W. Investigation on the porosity of
gel by thermal-desorption of liquids. Mater Chem Phys.
25. Goworek J, Stefaniak W. The porosity of solids by
orption of benzene. Charact Porous Solids Iii.
26. Gunko VM, Goncharuk OV, Goworek J. Evaporation of polar
and nonpolar liquids from silica gels and fumed silica.
Surf A. 2015;474:5262. doi:10.1016/j.colsurfa.2015.03.007.
27. Nita LE, Chiriac AP, Cimmino S, Silvestre C, Duraccio D,
C. Polymerization in magnetic field: XVIII. Influence of
tant nature on the synthesis and thermal properties of
methacrylate) and poly[(methyl methacrylate)-co-(epoxypropyl
methacrylate)]. Polym Int. 2008;57(2):3429. doi:10.1002/pi.
28. Podkoscielna B. The highly crosslinked
benzene copolymers Characterization and thermal studies.
J Therm Anal Calorim. 2011;104(2):72530. doi:10.1007/
29. de Oliveira HFN, Felisberti MI. Amphiphilic copolymers
sucrose methacrylate and acrylic monomers: bio-based
from renewable resource. Carbohyd Polym. 2013;94(1):31722.
30. Mohamed NA, Salama HE, Sabaa MW, Saad GR. Synthesis and
characterization of biodegradable
and their chitin whisker nanocomposites. J Therm Anal
31. Worzakowska M. Thermal behavior, decomposition mechanism
and some physicochemical properties of starch-g-poly(benzyl
acrylate) copolymers. J Therm Anal Calorim. 2016;126(2):
32. Worzakowska M. Starch-g-poly(benzyl methacrylate)
mers: characterization and thermal properties. J Therm Anal
Calorim. 2016;124(3):130918. doi:10.1007/s10973-016-5328-7.
33. Soppirnath KS, Aminabhavi TM. Water transport and drug
release study from cross-linked polyacrylamide grafted guar
hydrogel microspheres for the controlled release application.
J Pharm Biopharm. 2002;53(1):8798. doi:10.1016/S0939-
34. Yu YQ, Li ZZ, Tian HJ, Zhang SS, Ouyang PK. Synthesis
characterization of thermoresponsive hydrogels cross-linked
acryloyloxyethylaminopolysuccinimide. Colloid Polym Sci.
35. Janovak L, Varga J, Kemeny L, Dekany I. The effect of
modification of layer silicates on the thermoanalytical
of poly(NIPAAm-co-AAm) based composite hydrogels. J Therm
Anal Calorim. 2009;98(2):48593. doi:10.1007/s10973-009-
36. Yang JM, Chiu HC. Preparation and characterization of
alcohol/chitosan blended membrane for alkaline direct
fuel cells. J Membr Sci. 2012;419:6571.
37. Mittal H, Kaith BS, Jindal R, Mishra SB, Mishra AK. A
study on the effect of different reaction conditions on graft
merization, swelling, and thermal properties of Gum
hydrogels. J Therm Anal Calorim. 2015;119(1):13144.
38. Kuzema PO, Stavinskaya ON, Laguta IV, Kazakova OA. Ther-
mogravimetric study of water affinity of gelatin materials.
J Therm Anal Calorim. 2015;122(3):12317. doi:10.1007/
39. Passos MF, Dias DRC, Bastos GNT, Jardini AL, Benatti
Dias CGBT, et al. pHEMA hydrogels Synthesis, kinetics and
in vitro tests. J Therm Anal Calorim. 2016;125(1):3618.
Swelling effects in cross-linked polymers by thermogravimetry
Swelling effects in cross-linked polymers by
Results and discussionNitrogen adsorptionMicroscopic
studiesThermogravimetric experimentModel considerations